Gold(I)-Dithioether Supramolecular Polymers: Synthesis, Characterization, and Luminescence
Mohamed Osman Awaleh; François Baril-Robert; Christian Reber; Antonella Badia; François Brisse; Inorganic Chemistry 47 (2008) 2964–2974; doi:10.1021/ic701275k

data_4304025
_publ_contact_author_address
;
      Universit\'e de Montr\'eal
      D\'epartement de Chimie
      C.P. 6128, Succ. Centre-ville
      Montr\'eal, Qu\'ebec
      Canada, H3C 3J7
;
_publ_contact_author_email       francois.brisse@umontreal.ca
_publ_contact_author_fax         '+1 514 343 7586'
_publ_contact_author_name        'Dr Fran\,cois Brisse'
_publ_contact_author_phone       '+1 514 343 2088'
_publ_section_title
;
Gold(I)-Dithioether Supramolecular Polymers: Synthesis, Characterization,
and Luminescence
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2964
_journal_page_last               2974
_journal_paper_doi               10.1021/ic701275k
_journal_volume                  47
_journal_year                    2008
_chemical_compound_source        'Synthesized by the authors. See text'
_chemical_formula_moiety         'C8 H9 Au Cl S'
_chemical_formula_sum            'C8 H9 Au Cl S'
_chemical_formula_weight         369.63
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.620(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   11.9960(6)
_cell_length_b                   9.7548(5)
_cell_length_c                   8.5660(5)
_cell_measurement_reflns_used    6090
_cell_measurement_temperature    220(2)
_cell_measurement_theta_max      71.82
_cell_measurement_theta_min      3.87
_cell_volume                     955.35(9)
_computing_cell_refinement       'SMART (Bruker, 1999)'
_computing_data_collection       'SMART (Bruker, 1999)'
_computing_data_reduction        'SAINT (Bruker, 1999)'
_computing_molecular_graphics    'SHELXTL (Bruker, 1997)'
_computing_publication_material  'UdMX (local program)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      220(2)
_diffrn_detector_area_resol_mean 5.5
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker Smart 2000'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Sealed Tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.074
_diffrn_reflns_av_sigmaI/netI    0.0609
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            10839
_diffrn_reflns_theta_full        72.02
_diffrn_reflns_theta_max         72.02
_diffrn_reflns_theta_min         3.87
_diffrn_standards_decay_%        0.44
_diffrn_standards_number         68
_exptl_absorpt_coefficient_mu    33.008
_exptl_absorpt_correction_T_max  0.262
_exptl_absorpt_correction_T_min  0.103
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Sadabs (Sheldrick,1996)'
_exptl_crystal_colour            Colourless
_exptl_crystal_density_diffrn    2.570
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle-like
_exptl_crystal_F_000             676
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.04
_refine_diff_density_max         2.144
_refine_diff_density_min         -1.952
_refine_diff_density_rms         0.330
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.021
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     100
_refine_ls_number_reflns         1871
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.021
_refine_ls_R_factor_all          0.0561
_refine_ls_R_factor_gt           0.0538
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1044P)^2^+0.9689P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1338
_refine_ls_wR_factor_ref         0.1371
_reflns_number_gt                1709
_reflns_number_total             1871
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            ic701275k-file.008.cif
_cod_data_source_block           Complex7
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_geom_angle_publ_flag' value 'Y' changed to 'y' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (14
times).

'_geom_bond_publ_flag' value 'Y' changed to 'y' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (12 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4304025